Welding Research Sponsored by the Welding Research Council
SUPPLEMENT TO THE WELDING JOURNAL, DECEMBER 1972
Procedures for Evaluation of Fracture Toughness of Heat-Affected Zones
BY L. J . McGEADY
A good quality weld requires adequate fracture tough-ness of base metal, weld metal, and heat-affected zone (HAZ). Reliable methods are available for the first two but the HAZ evaluation has posed particular experi-mental problems which are dealt with in this paper.
In t roduct ion
Welded structures must be viewed essentially as three-component com-posites of weld metal, plate and heat-affected zone (HAZ). Inadequate toughness in any one is a threat to structural integrity.
In carbon steel weldments the frac-ture situation is generally a plate problem in the main. The protective geometric aspects of U- or Vee-groove geometries and the toughness levels in welds deposited wi th modest control generally el iminate the HAZ and weld metal as common paths of major failure. However f laws in either area are capable of exten-sion to the plate. Therefore the key to catastrophic fracture control has cen-tered on the use of steel of sufficient-
L. J. McGeady is professor and head of the Department of Metallurgical Engineering at Lafayette College, Easton, Pa.
ly low transit ion temperature. The World War II ship failure problem is an excellent case for reference.
In weldments of quenched and tem-pered steels, the potential for ex-tended fractures not only in plate but also in either HAZ or weld metal must be considered. The steels in this group, because of differences in alloy content and kind differ widely in plate toughness characteristics and in sensitivity to HAZ damage in welding. At the same t ime the higher strength requirements for weld metals for these steels pose considerations in respect to toughness wh ich become more acute as advanced strengths or more economic compositions or both are sought.
The control of fracture via the plate transit ion temperature wh i le possible for carbon steel weldments is insuf-f icient for quenched and tempered steel weldments. Evaluative methods for the quenched and tempered (Q+T) steel must take into account the sus-
ceptibility of all weldment com-ponents to fracture. Two approaches are possible. Testing weldments in composite specimen procedures such as the Explosion Bulge or Delta allows identification of the most frac-ture prone elements. Procedures to test the toughness of the weld, plate and HAZ represent a second ap-proach.
The Drop-Weight (DW) and Dynam-ic Tear (DT) tests have been used widely to characterize plate and weld metal toughness separately and quantitatively. From tests using these two specimens, data are presented in this report to demonstrate the ap-plicability of these two procedures to the HAZ as wel l . Results of composite specimen tests and single component tests wi l l be shown to be in agree-ment when applied to several steels. Consequently the understanding of results of composite specimens tests is enhanced and their applicability better defined. At the same t ime the
W E L D I N G R E S E A R C H S U P P L E M E N T ! 569-s
successful characterization of HAZ toughness by the DW and DT procedures provides quantitative ref-erence data for use in the Fracture Analysis and Ratio Analysis Dia-grams.
T h e Weldab i l i ty Prob lem in Relat ion to Fracture Toughness in C a r b o n Stee ls
The ship failures in Wor ld War II typified the weldabil i ty problem in carbon steel structures. The intensive investigation of these failures re-vealed that the fracture problem was essentially a plate metal problem, that is, high plate transit ion temper-atures, since they were the path for extended failures. Adequate tough-ness in the weld metal was possible through use of commercial fi l ler ma-terials deposited under modest con-trol. Sufficient compensation for met-allurgical damage via the protective geometric aspects of joints w i th U-or Vee-groove configurations was ef-fective in minimizing extended frac-tures in the HAZ.
However f laws in either the weld metal or heat-affected zone could and did act as sources for fractures which were transmitted to and extended in the plate. As a consequence a two-pronged attack was brought to bear on the carbon steel fracture problem one, to produce plate w i th lower transit ion temperatures, the other to identify and el iminate creation of f laws in welding.
In the effort, a host of tests was developed. In the context of the prob-lem, all were called weldabil i ty tests. Some were designed to measure plate toughness more satisfactorily or completely than possible by the Charpy test; these were regarded as service tests. Others gene ra l l y termed fabrication tests were de-signed to measure susceptibility of the base plate to heat-affected zone cracking. One was the bead on plate cracking test in wh ich a weld bead was deposited on the plate material and then examined for evidence of cracking in the HAZ under the natural shrinkage stresses generated by weld cooling.
A second procedure was the "c l ip test " in which a piece of plate or " c l i p " was welded w i th a single f i l let weld to form a Tee-joint w i th the material being examined. Testing consisted of striking the clip, which was the vertical bar of the Tee-joint, w i th a sledge to determine whether in breaking it away, fracture took place in the brittle coarse-grained HAZ of the subject material.
Another approach to determine susceptibility of either weld metal or HAZ to cracking in fabrication was the Lehigh Restraint1 Specimen. In
this test, a weld deposited in a double-U-joint was restrained from shrinking in cooling. Variable restraint al lowed definit ion of a threshold value above which cooling cracks would form. Either weld metal or HAZ could fail depending on the materials and weld-ing conditions.
Consideration of the HAZ as an area of potential difficulty led to vari-ous researches. Doan, Stout, Tor and Frye2 proposed a systematic ap-proach to controll ing hardness and britt leness in the coarse-grain heat-affected zone through understanding the relations between weld heat input, plate thickness and temper-ature, and corresponding cooling rates in the weld area and Jominy test data. Other i nves t i ga t i ons showed potential embri t t lement in re-gions of the HAZ susceptible to strain-aging type phenomena. Stil l others showed embrit t lement possible in the metallurgical areas heated just above the lower critical temperature.
However, the situation w i th the car-bon steel plates remained the same, namely the potential for long disas-trous failures in plate w i th the weld zone l imited to the role of site or source of init iat ion. Commercial weld-ing material and control of welding conditions could be relied on to el im-inate the weld zones as paths for major fracture. Ult imately it became clear that the overall approach to frac-ture safe design w i th these steels re-quired the use of sufficiently low t ran-sition temperature plate material to prevent extensive fracture.
Weldabi l i ty and Fracture Toughness of H i g h - S t r e n g t h Stee ls
Weldabil i ty is a more complex prac-tical matter for the high-strength steels than for the carbon steels. Not only the plate but also the heat-affected zone and the weld metal re-quire consideration. Each can be viewed as a separate concern.
Conceptually and for practical test-ing purposes the weld metal is isola-ble for separate handling. However the fracture toughness problems there must be considered in relation to the steels being welded. For car-bon steels the problem is minimal. Adequate toughness or toughness equivalent to that of the plate is read-ily obtained in the weld metal w i th relatively modest attention to the welding process using readily avail-able fi l ler materials. Welding of high-strength steels presents more str in-gent demands. As in the plate materi-als to wh ich they are applied the prob-lem is to maintain adequate tough-ness at elevated strength levels. Thus the weld metal toughness problem becomes more acute as higher
strengths or more economic composi-tions or both are sought. Optimum properties are realized only by careful selection of fil ler material and appro-priate control of the welding process.
Like the weld metal, plate material can be handled as a distinctly sep-arate weldment component. It is clearly recognized that differences in amount and kind of a l loyirg elements lead to differences in toughness char-acteristics at any strength level. Some of the steels in the Q+T group show neither a sharp transit ion tem-perature nor a high energy shelf whi le others do. It is evident that in Q+T steel weldments the plate re-mains a critical element for fracture control.
Whi le the plate metal and HAZ can be viewed as separate entit ies, the plate must be regarded as the parent of the HAZ. Both are subject to the same metallurgical considerations. The fracture toughness realizable in each is dependent upon the nature and level of alloy content. The plate is heat treated for opt imum toughness in prescribed thermal cycling pro-cesses under control in the mil l . The more complex cycling experienced in the heat-affected zone is subject to less control in welding. It is unrealis-tic to expect the heat-affected zone to exhibit the same microstructures found in the plate. Control of the welding process must be the route to produce HAZ microstructures w i th op-t imum properties in a given steel. In general the hardenability of the steel dictates the latitude of welding condi-tions allowable for retention of the most favorable HAZ microstructure w i th resultant minimal damage.
Weldabi l i ty Tests
Among the various procedures pro-posed for